#------------------------------------------------------------------------------
#$Date: 2021-07-05 19:10:48 +0200 (lun 05 de jul de 2021) $
#$Revision: 267123 $
#$URL: svn://www.crystallography.net/cod/cif/7/24/28/7242875.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7242875
loop_
_publ_author_name
'Richardson, Jonathan G.'
'Mizuno, Asato'
'Shuku, Yoshiaki'
'Awaga, Kunio'
'Robertson, Neil'
'Morrison, Carole A.'
'Warren, Mark R.'
'Allan, David R.'
'Moggach, Stephen A.'
_publ_section_title
;
 Evaluating the high-pressure structural response and crystal lattice
 interactions of the magnetically-bistable organic radical TTTA
;
_journal_issue                   25
_journal_name_full               CrystEngComm
_journal_page_first              4444
_journal_page_last               4450
_journal_paper_doi               10.1039/D1CE00577D
_journal_volume                  23
_journal_year                    2021
_chemical_formula_moiety         'C2 N3 S3'
_chemical_formula_sum            'C2 N3 S3'
_chemical_formula_weight         162.24
_space_group_IT_number           14
_space_group_name_Hall           '-P 2ybc'
_space_group_name_H-M_alt        'P 1 21/c 1'
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     direct
_audit_creation_date             2021-04-22
_audit_creation_method           CRYSTALS_ver_14.61_build_6999
_audit_update_record
;
2021-04-27 deposited with the CCDC.	2021-05-18 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 104.34(5)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.280(10)
_cell_length_b                   3.3957(3)
_cell_length_c                   14.640(3)
_cell_measurement_reflns_used    888
_cell_measurement_temperature    293
_cell_measurement_theta_max      19
_cell_measurement_theta_min      4
_cell_volume                     447.0(5)
_computing_cell_refinement       'USER DEFINED CELL REFINEMENT'
_computing_data_collection       'USER DEFINED DATA COLLECTION'
_computing_data_reduction
; 
 CrysAlisPro (Rigaku Oxford Diffraction, 2017) 
;
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'SHELXS 86 (Sheldrick, 1986)'
_diffrn_ambient_pressure         2110000
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.344
_diffrn_measured_fraction_theta_max 0.337
_diffrn_measurement_device       Area
_diffrn_measurement_device_type  Synchrotron
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  'focussing mirrors'
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.48590
_diffrn_reflns_av_R_equivalents  0.019
_diffrn_reflns_av_unetI/netI     0.029
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -4
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            1902
_diffrn_reflns_theta_full        14.322
_diffrn_reflns_theta_max         18.845
_diffrn_reflns_theta_min         3.850
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.505
_exptl_absorpt_correction_T_max  0.95
_exptl_absorpt_correction_T_min  0.76
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'DENZO/SCALEPACK (Otwinowski & Minor, 1997)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.411
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             324
_exptl_crystal_size_max          0.120
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.31
_refine_diff_density_min         -0.38
_refine_ls_extinction_method     None
_refine_ls_goodness_of_fit_ref   1.0345
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     73
_refine_ls_number_reflns         374
_refine_ls_number_restraints     104
_refine_ls_R_factor_all          0.0490
_refine_ls_R_factor_gt           0.0396
_refine_ls_shift/su_max          0.0003774
_refine_ls_shift/su_mean         0.0000218
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 Method= Modified Sheldrick 
 w=1/[σ²(F²) + ( 0.05P)² + 2.64P] 
 ,where P=(max(Fo²,0) + 2Fc²)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1103
_refine_ls_wR_factor_gt          0.1041
_refine_ls_wR_factor_ref         0.1103
_reflns_limit_h_max              4
_reflns_limit_h_min              -6
_reflns_limit_k_max              4
_reflns_limit_k_min              0
_reflns_limit_l_max              17
_reflns_limit_l_min              0
_reflns_number_gt                303
_reflns_number_total             374
_reflns_threshold_expression     I>2.0σ(I)
_oxford_diffrn_Wilson_B_factor   0.00
_oxford_diffrn_Wilson_scale      0.00
_oxford_refine_ls_r_factor_ref   0.0490
_oxford_refine_ls_scale          0.761(6)
_oxford_reflns_number_all        374
_cod_data_source_file            d1ce00577d2.cif
_cod_data_source_block           211GPa
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_exptl_crystal_density_meas' value 'not measured' was
changed to '?' -- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 

 Adding full bibliography for 7242874--7242883.cif.
;
_cod_original_cell_volume        446.9(5)
_cod_original_sg_symbol_H-M      'P 1 21/c 1 '
_cod_database_code               7242875
_oxford_refine_reflns_threshold_expression_ref I>-10.0\s(I)
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
-x,y+1/2,-z+1/2
x,-y+1/2,z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
_atom_site_attached_hydrogens
S1 S 0.4397(4) 0.2975(5) 0.33830(13) 0.0392 1.0000 Uani D U . . . .
N2 N 0.3143(8) 0.1837(13) 0.2402(3) 0.0400 1.0000 Uani D U . . . .
S3 S 0.1459(4) 0.0681(4) 0.25003(11) 0.0346 1.0000 Uani D U . . . .
C4 C 0.1781(8) 0.1246(13) 0.3714(3) 0.0296 1.0000 Uani D U . . . .
C5 C 0.3267(7) 0.2417(13) 0.4158(3) 0.0268 1.0000 Uani D U . . . .
N6 N 0.3512(8) 0.2941(12) 0.5075(3) 0.0312 1.0000 Uani D U . . . .
S7 S 0.1943(4) 0.1825(4) 0.53573(11) 0.0304 1.0000 Uani D U . . . .
N8 N 0.0918(8) 0.0728(13) 0.4296(3) 0.0308 1.0000 Uani D U . . . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
C 0.0006 0.0007 2.3100 20.8439 1.0200 10.2075 1.5886 0.5687 0.8650 51.6512
0.2156 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
N 0.0016 0.0014 12.2126 0.0057 3.1322 9.8933 2.0125 28.9975 1.1663 0.5826
-11.5290 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
S 0.0630 0.0572 6.9053 1.4679 5.2034 22.2151 1.4379 0.2536 1.5863 56.1720
0.8669 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_site_symmetry_1
_geom_angle_atom_site_label_2
_geom_angle_site_symmetry_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
N2 . S1 . C5 . 97.7(3) yes
S1 . N2 . S3 . 117.1(3) yes
N2 . S3 . C4 . 97.8(3) yes
S3 . C4 . C5 . 113.5(4) yes
S3 . C4 . N8 . 131.9(4) yes
C5 . C4 . N8 . 114.6(4) yes
C4 . C5 . S1 . 113.9(3) yes
C4 . C5 . N6 . 113.9(4) yes
S1 . C5 . N6 . 132.2(4) yes
C5 . N6 . S7 . 106.5(4) yes
N6 . S7 . N8 . 98.9(3) yes
C4 . N8 . S7 . 106.1(4) yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_site_symmetry_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
S1 . N2 . 1.655(6) yes
S1 . C5 . 1.735(5) yes
N2 . S3 . 1.653(7) yes
S3 . C4 . 1.738(4) yes
C4 . C5 . 1.427(7) yes
C4 . N8 . 1.318(6) yes
C5 . N6 . 1.318(5) yes
N6 . S7 . 1.653(7) yes
S7 . N8 . 1.651(5) yes
